Electrolessly Deposited Electrospun Metal ... Electrolessly Deposited Electrospun Metal Nanowire...
Embed Size (px)
Transcript of Electrolessly Deposited Electrospun Metal ... Electrolessly Deposited Electrospun Metal Nanowire...
Electrolessly Deposited Electrospun Metal Nanowire Transparent Electrodes Po-Chun Hsu,† Desheng Kong,† Shuang Wang,‡ Haotian Wang,§ Alex J. Welch,† Hui Wu,†,⊥
and Yi Cui*,†,∥
†Department of Materials Science and Engineering, ‡Department of Electrical Engineering, and §Department of Applied Physics, Stanford University, Stanford, California 94305, United States ∥SLAC National Accelerator Laboratory, Stanford Institute for Materials and Energy Sciences, Menlo Park, California 94025, United States
*S Supporting Information
ABSTRACT: Metal nanowire (MNW) transparent elec- trodes have been widely developed for their promising sheet resistance (Rs)−transmittance (T) performance, excellent mechanical flexibility, and facile synthesis. How to lower the junction resistance without compromising optical transmittance has become the key issue in enhancing their performance. Here we combine electro- spinning and electroless deposition to synthesize inter- connected, ultralong MNW networks. For both silver and copper nanowire networks, the Rs and T values reach around 10 Ω/sq and 90%, respectively. This process is scalable and takes place at ambient temperature and pressure, which opens new opportunities for flexible electronics and roll-to-roll large-scale manufacturing.
Transparent conducting electrodes (TCEs) are indispen-sable components in many optoelectronic devices such as displays, light-emitting diodes (LEDs), touchscreens, smart windows, and solar cells.1 It is important to develop transparent electrodes with low sheet resistance (Rs) at high transmittance (T) to decrease the ohmic loss of the electronic circuit while maintaining good transparency. Currently the dominant material for TCE is indium tin oxide (ITO), but its high cost and brittleness limit its applications.2 Various alternative TCEs are being developed such as conducting polymers,3 carbon nano- tubes,4 graphenes,5 and metal nanowire (MNW) networks.6
Among these novel TCEs, MNW networks are particularly promising because of their high electrical conductivity; intensive research efforts have been focused on enhancing their Rs−T performance. Recently the mesoscale metal wire concept was combined with MNW networks to further reduce Rs by an order of magnitude.7 Key issues to address for MNW TCEs are junction resistance and the number of junctions that conducting pathways encounter.8 Junction resistance can be greatly decreased by post-treatments such as thermal annealing,6d wet chemical coating,8 nanoplasmonic welding,9 and electroweld- ing;10 however, these often limit the use of substrates and increase the process complexity. To decrease the number of junctions, longer NWs must be synthesized: longer NWs not only require fewer junctions to reach the contact pad but also lower the percolation threshold Nc, expressed as √(πNc) = 4.236/L,4c where L is the length of NWs. It is clear that for longer
NWs, Nc is lower, and the probability of having a continuous pathway becomes higher, resulting in lowerRs. The best solution- processed MNWTCEs are reported to have Rs and T values of 9 Ω/sq and 89%, respectively, for silver nanowires (AgNWs)9b and 40 Ω/sq and 90%, respectively, for copper nanowires (CuNWs).11 Here, we propose a novel method to synthesize interconnected, ultralong, high-performance MNWs at ambient temperature and pressure, which is suitable for flexible and soft substrates. By using electrospinning and electroless deposition, we are able to solve both junction resistance and NW length issues. This approach produces MNWs that are low-cost and scalable but also have decent Rs−T performance. The process flow of electrolessly deposited metallic electro-
spun NWTCEs is shown in Figure 1. Essentially, the electrospun
polyvinyl butyral (PVB) NWs network was used as the template for electroless metal deposition. Electrospinning produces ultralong NWs12 that provide continuous pathways for electron transport after metallization of the NW network. Electroless deposition is a well-established technique for depositing metal films at low cost and large scale. In combination, these two methods offer a cost-effective way to make MNW networks. To guarantee great Rs−T performance, it is necessary to selectively deposit metal on the PVB NWs instead of the substrate. This
Received: June 12, 2014
Figure 1. Schematic of electrolessly deposited metallic electrospun nanowire transparent electrodes. PVB/SnCl2 NWs were electrospun onto a glass slide spin-coated with hydrophobic PVB thin film, followed by immersion into AgNO3 solution to form a Ag catalyst seed layer. The sample was then rinsed and transferred to electroless deposition solution to form Ag or Cu NWs.
© XXXX American Chemical Society A dx.doi.org/10.1021/ja505741e | J. Am. Chem. Soc. XXXX, XXX, XXX−XXX
issue is tackled by two key steps in our method. First, tin(II) chloride is dissolved in the PVB solution, electrospun as PVB/ SnCl2 NWs. When the NWs are immersed in silver nitrate aqueous solution, Ag+ is reduced by Sn2+ and forms a Ag seed layer on the surface, which acts as the catalytic nucleation site for Ag or Cu electroless deposition.13 Second, the substrates are spin-coated with hydrophobic polymer film before the PVB nanofiber electrospinning, so it is more energetically unfavorable for metal precursors to be reduced onto the substrates. Here we also use PVB for the hydrophobic coating. The electrospun PVB/SnCl2 NWs are characterized by X-ray
photoelectron spectroscopy (XPS) before and after AgNO3 treatment (Figure 2a). For the as-electrospun NWs, the Sn 3d5/2 peak was deconvoluted and fitted as two subpeaks at 487.0 and 488.7 eV. According to previous XPS research,14 the lower binding energy subpeak (487.0 eV) corresponds to the SnCl2
dispersed in the NW, while the higher binding energy subpeak might correspond to SnO2 or Sn(OH)4 impurities due to oxidation of Sn2+ species when exposed to ambient atmos- phere.15 After AgNO3 treatment, Sn
2+ is expected to be oxidized to Sn4+, and Ag seeds should appear and bind to the NW surface, as indicated by the Ag 3d5/2 peak. The XPS result again agrees very well with the literature,14 showing a 0.8 eV shift toward lower binding energy down to 486.2 eV for the Sn 3d5/2 peak. The XPS study supports the use of SnCl2 and AgNO3 as reagents to provide a Ag seed layer to catalyze the subsequent electroless deposition. Systematic characterizations reveal the morphology and
composition of the as-synthesized NW network. Figure 2b,c shows the scanning electron microscopy (SEM) image and the corresponding energy-dispersive spectroscopy (EDS) elemental map of electrolessly deposited AgNWs and CuNWs, respec- tively. The red color in the EDS represents AgL characteristic radiation, and green represents CuK. Apparently, the substrate passivated by hydrophobic coating is free of metal deposition, and the Ag seed catalysts successfully facilitate metallization on the polymer NWs. For TCE applications, the NWs used in our study are generally 200 nm in diameter. With the diameter of electrospun NWs being ∼60 nm (Figure S1), the thickness of metal deposition is ∼70 nm. We intentionally reduce the diameter of PVB NWs as much as possible, since the polymer cores of the NWs do not contribute to the electrical conductance. The thickness of MNWs must also be carefully chosen. Thin deposition gives smaller crystal grains and therefore more defects or voids, while thick deposition reduces the optical transmittance compared to the thin counterpart, given the same NW density. We found that a 70 nm thickness guarantees complete metallization coverage as well as high optical transmittance. The time dependence of the thickness of CuNWs is shown in
Figure 2d. The growth exhibits an induction period followed by a linear increase in the thickness. This behavior agrees well with the mixed-potential theory,16 in which the induction period is the duration until the reducing agent and the metal ions reach the same potential before deposition occurs. The chemical equations for Cu electroless deposition by dimethylamine borane (DMAB) are illustrated in Scheme 1.
During the incubation period, the Ag catalyst seed layer facilitates oxidization of DMAB to reach the same potential as the metal precursors, and thus steady-state electroless deposition can occur. It is worth noting that the incubation time significantly depends on the atmosphere and stirring rate,17 so good control of the oxygen partial pressure and stirring environment is important to guarantee uniformity and reproducibility. Figure 3a shows the Rs−T relationships of our electrolessly
deposited MNWs, which are controlled by the electrospinning time and resulting NW areal density. To our knowledge, this Rs− T performance (8.5 Ω/sq and 90% for AgNWs, 11.2 Ω/sq and
Figure 2. (a) XPS spectra of nanowires as-electrospun and after AgNO3 treatment, referenced to C 1s at 284.5 eV. (b,c) SEM and EDS mapping of Ag and Cu NWs on glass substrates, respectively. The scale bars are 2 μm. Note that there is no conductive coating for imaging, so the substrates are insulating and cause charging effect between the NWs. (d) CuNW diameter vs electroless deposition time. The diameter of the electrospun PVB/SnCl2 NWs is ∼60 nm. The electroless deposition exhibits an induction time of ∼30 min, followed by a constant-rate deposition. The blue dashed line is a guide.
Scheme 1. Copper Electroless Deposition in Alkaline Solution Using EDTA as Chelating Agent and DMAB as Reducing Agent
Journal of the American Chemical Society Communication
dx.doi.org/10.1021/ja505741e | J. Am. Chem. Soc. XXXX, XXX, XXX−XXXB